ARCHIVES of

Computational Materials Science and Surface Engineering

International Scientific Journal published quarterly by the Association of Computational Materials Science and Surface Engineering

2 0 0 9 • Vo l u m e 1 • Is s ue 3 • 133- 138

Application of artificial neural network for predicting fatigue crack propagation life of aluminum alloys J.R. Mohanty *, B.B. Verma, D.R.K. Parhi, P.K. Ray

Department of Metallurgical and Materials Engineering, National Institute of Technology, Rourkela 769008, India * Corresponding author: E-mail address: [email protected] Received in a revised form 08.05.2008

ABSTRACT

Purpose: In this work, fatigue crack propagation life of 7020 T7 and 2024 T3 aluminum alloys under the influence of load ratio was predicted by using artificial neural network (ANN). Design/methodology/approach: Numerous phenomenological models have been proposed for predicting fatigue life of the components under the influence of load ratio to take into account the mean load effect. Findings: In current research, an automatic prediction methodology has been adopted to estimate the constant amplitude loading fatigue life under the above condition by applying artificial neural network (ANN). Practical implications: ANNs show great potential for predicting fatigue crack growth rate especially by interpolation within the tested range. However, its benefit is lost when the model is needed to extrapolate the available experimental data. Originality/value: The predicted results are found to be in good agreement with the experimental findings when tested on two aluminum alloys 7020 T7 and 2024 T3 respectively. Keywords: Fatigue crack growth rate; Artificial Neural Network; Constant amplitude loading Reference to this paper should be given in the following way: J.R. Mohanty, B.B. Verma, D.R.K. Parhi, P.K. Ray, Application of artificial neural network for predicting fatigue crack propagation life of aluminum alloys, Archives of Computational Materials Science and Surface Engineering 1/3 (2009) 133-138.

ENGINEERING MATERIALS

1. Introduction 1. Introduction Most load bearing structural components generally contain defects / imperfections either as a result of manufacturing, fabrications or localized damage in service. Under different loading conditions, these defects coalesce and develop into large cracks, which propagate to critical size resulting catastrophic failure. The mere presence of a crack does not make a component or structure to be unreliable. Whatever may be the loading

condition, whether cyclic or sustained loading, it is necessary to know how long a crack would take to grow to a critical size at which the component or structure would become unsafe and fail. Therefore, the crack growth studies and life prediction procedure under fatigue loading is essential in order to extend the life of inservice sophisticated components so as to provide huge savings. It is known that load ratio (R) has a marked effect on fatigue crack growth rate. During last four decades, many prediction models have been proposed to incorporate the effect of R-ratio

© Copyright by International OCSCO World Press. All rights reserved. 2009

133

J.R. Mohanty, B.B. Verma, D.R.K. Parhi, P.K. Ray

including crack closure model [8], models based on residual compressive stress [13,15,] two-parameter driving force models [6,14] etc. However, automatic life prediction based on softcomputing methods such as artificial neural network (ANN), genetic algorithm (GA) etc is lacking. In the current investigation, an attempt has been made to predict fatigue life under the influence of R-ratio by using ANN. It is observed that the predicted results are in good agreement with the experimental findings.

K

f ( g ).

F Sa wB

(1)

where, f(g) = 1.12-0.231(a/w)+10.55(a/w)2-21.72(a/w)3+30.39(a/w)4 (2)

2. Experimental procedure 2. Experimental procedure This research was carried out on 7020 T7 and 2024 T3 aluminum alloys. A summary of chemical compositions and mechanical properties of both the alloys have been presented in Tables 1 and 2 respectively. The fatigue crack growth tests were performed using single edge notch tension (SENT) specimen with a thickness of 6.48 mm. The specimens were made in the LT plane, with the loading aligned in the longitudinal direction. Fig. 1 illustrates the major dimensions of the SENT samples used in the tests. A servo-hydraulic dynamic testing machine (Instron-8502) having a load capacity of 250 KN was used for the present investigation. Fatigue pre-cracking was introduced under mode I loading condition to an a/w ratio of 0.3 and were subjected to constant load amplitude test maintaining six load ratios (R) of 0, 0.2, 0.4, 0.6 and 0.8 respectively for both the materials. All fatigue tests were run at a frequency of 6 Hz with a sinusoidal wave form under ambient laboratory condition. Crack lengths were measured using a compliance method with a COD gauge and were also controlled using an optical method with a 20X magnification. The stress intensity factors at every instant ahead of the crack tip were calculated by using the following equations [4]:

Fig. 1. Geometry of the SENT specimen (dimensions in mm)

Table 1. Chemical Composition of 7020 T7 and 2024 T3 aluminum alloys Materials Al Cu Mg Mn 7020 T7 Main 0.05 1.2 0.43 constituent 2024 T3 90.7– 94.7 3.8 – 4.9 1.2–1.8 0.3 – 0.9

Table 2. Mechanical Properties of 7020 T7 and 2024 T3 aluminum alloys Young’s modulus Materials Tensile strength Yield strength (ıys) (E) (ıut) MPa MPa MPa

Fe 0.37

Si 0.22

Zn 4.6

Cr -

Others -

0.5

0.5

0.25

0.1

0.15

Poisson’s ratio (Ȟ)

Plane Strain Fracture toughness (KIC)

Elongation

MPa m 7020 T7

352.14

314.70

70,000

0.33

50.12

2024 T3

469.00

324.00

73,100

0.33

37.00

134

21.54 % in 40 mm 19 % in 12.7 mm

Archives of Computational Materials Science and Surface Engineering

Application of artificial neural network for predicting fatigue crack propagation life of aluminum alloys

3. Artificial neural 3. Artificial neuralnetwork networkapproach approach Artificial neural network (ANN) is a new class of computational intelligence system, useful to handle various complex problems with a capacity to learn by examples. It has proved to be a powerful and versatile soft-computing method which is quite efficient in modeling complex linear and non-linear relationships on the basis of experimental data in a number of engineering fields [1,3,11,16,18]. In recent years, ANN finds its application in the field of fatigue for various purposes [2,5,9,12,19,20,22]. It can be categories as feed forward or recurrent depending on the processing of data through the network. According to the learning rules, it can be further classified as supervised, unsupervised or reinforcement ANN. Among the various classifications, multi-layer perceptron (MLP) is the most popular ANN architecture as far as engineering application is concerned. MLPs are generally used with feed forward neural networks trained with error-back propagation algorithm (error minimization technique). Various non-linear activation functions such as sigmoidal, tanh or radial (Gaussian) are used to model the neuron activity.

4. esign ofofanan ANN model for crack 4. D Design ANN model for crack growth rate prediction growth rate prediction In the present investigation, a nine-layer perceptron ANN with back-propagation neural controller [10] has been developed. It has got one input layer, one output layer and seven hidden layers. The input layer has got three neurons, whereas one neuron has been associated with output layer. The neurons associated in the seven hidden layers are twelve, twenty four, hundred, thirty five and eight respectively. The neurons have been chosen empirically and taken in order so as to give the neural network a diamond shapes (Fig. 2).

The input parameters to the neural network controller are as follows: Stress intensity factor range = “sifr”; Maximum stress intensity factor = “msif”; Load ratio = “lr”. The output from the controller is: Crack growth rate = “cgr” The proposed ANN has been written in the C++ programming language and all the training tests have been performed on a personal computer. The activation function chosen in this work is the hyperbolic tangent function:

f ( x)

ex ex e x e x

(3)

During training, the network output șactual, may differ from the desired output șdesired as specified in the training pattern presented to the network. A measure of the performance of the network is the instantaneous sum-squared difference (error) between șdesired and șactual for the set of presented training patterns: 2 1 E rr ¦ T desired T actual 2 all training patterns

(4) where șactual represents crack growth rate (“cgr”) The two crack driving forces: stress intensity factor range (ǻK) and maximum stress intensity factor (Kmax) have been chosen as the two inputs as per ‘Unified Approach’ [6,7,14,21]. The third input is the load ratio (R) as the fatigue crack growth rate (da/dN) varies with the load ratio. The crack growth rate has been chosen as the output for the present ANN model. As far as normalization of input and output parameters are concerned, classical normalization, where the range is scaled between 0 and 1, may not be applicable in every ANN model. To make the input amenable for successful learning to minimize the overall sumsquared error, the two input parameters ǻK and Kmax have been normalized between 1 and 4, while the other one, load ratio (R) has been normalized between 1 and 3. Similarly the output § d a · ¨ ¸ © dN ¹

has been normalized between 0 and 3 for network training and testing. The inputs and outputs of the training sets (TS) have been constituted from 3× 65 experimental values of ǻK, Kmax and § da · data for each of the load ratios 0, 0.2, 0.4, 0.6, and 0.8 for ¨ ¸ © dN ¹ both the alloys.

5. Results 5. Results 5.1. Experimental 5.1 Experimentalresults results The experimental values of crack length versus number of cycles for various load ratios (R) have been illustrated in Figs. 3 and 4 respectively for both the materials. The crack growth rate,

§ da · has been calculated by incremental polynomial method as ¨ ¸ © dN ¹ Fig. 2. ANN architecture

Volume 1 • Issue 3 • 2009

per ASTM1. The results have been plotted against stress intensity factor (ǻK) in Figs. 5 and 6.

135

J.R. Mohanty, B.B. Verma, D.R.K. Parhi, P.K. Ray

36

R=0 R=0.2 R=0.4 R=0.5 R=0.6 R=0.8

34 32

28

0.95

1.05

1.15

1.25

1.35

1.45

1.55

-2.1

-2.6

log(da/dN)

Crack length(a),mm

30

0.85

26 24

-3.1

22

R=0

-3.6

R=0.2

20

R=0.4

18 16 3.00E+04 4.00E+04 5.00E+04 6.00E+04 7.00E+04 8.00E+04 9.00E+04 1.00E+05

-4.6

Fig. 3. Comparison of a ~ N curves for different load ratios (7020 T7 alloy) 36

30 28

Fig. 6. Comparison of da/dN ~ ǻK curves for different load ratios (2024-T3 alloy)

C rac k grow th rate(da/dN ).m m /c yc le

32

26 24 22 20 18 16 7.00E+04

log(del.K

2.00E-02

R=0 R=0.2 R=0.4 R=0.5 R=0.6 R=0.8

34

R=0.6 R=0.8

No. of cycle(N)

Crack length(a),mm

R=0.5

-4.1

9.00E+04

1.00E+05

1.10E+05

1.20E+05

Experimental

1.60E-02 1.40E-02 1.20E-02 1.00E-02 8.00E-03 6.00E-03 4.00E-03 2.00E-03 0.00E+00

8.00E+04

Predicted

1.80E-02

1.30E+05

10

15

No. of cycle(N)

Fig. 4. Comparison of a ~ N curves for different load ratios (2024 T3 alloy)

1.1

1.2

1.3

1.4

1.5

1.6

-1.7

log(da/dN)

-2.2

-2.7

-3.2

R=0

R=0.2

-3.7

R=0.4 R=0.5

-4.2

R=0.6 R=0.8

-4.7

log(del.K)

Fig. 5. Comparison of da/dN ~ ǻK curves for different load ratios (7020-T7 alloy)

136

Crack growth rate(da/dN),mm/cycle

1

25

30

35

Figure 7. Comparison of predicted (ANN) and experimental crack growth rate with stress intensity range (¨K) for load ratio 0.5 (7020 T7 alloy) 2.00E-02

0.9

20

Stress intensity factor range(del.K),Mpa.m^1/2

Predicted

1.80E-02

Experimental

1.60E-02 1.40E-02 1.20E-02 1.00E-02 8.00E-03 6.00E-03 4.00E-03 2.00E-03

0.00E+00

8.5

13.5

18.5

23.5

28.5

Stress intensity factor range(del.K),Mpa.m^1/2

33.5

Fig. 8.Comparison of predicted (ANN) and experimental crack growth rate with stress intensity range (¨K) for load ratio 0.5 (2024 T3 alloy)

Archives of Computational Materials Science and Surface Engineering

Application of artificial neural network for predicting fatigue crack propagation life of aluminum alloys

Table 3. Load scenarios and model results of the tested specimens Test specimen Fmax Fmin R ai (KN) (KN) (mm)

af (mm)

N Af

N Ef

% error in

% error in

Kcycle

Kcycle

N Af

N Ef

7020 T7

7.944

3.972

0.5

18.3

35.1

75.344

78.265

-4.365

-0.658

2024 T3

7.204

3.602

0.5

18.3

35.4

110.920

112.879

-2.099

-0.370

34

hidden neurons, minimum error and number of iterations were chosen empirically as 7, 1 u 10 6 and 4, 48, 000. The input parameters, stress intensity factor range (ǻK), maximum stress intensity factor (Kmax) and load ratio have been fed to the trained ANN model in order to predict the corresponding crack growth

Predicted

Experimental

Crack length(a),mm

32 30 28

rate §¨ da ·¸ for the validation set. The predicted crack growth

26

© dN ¹

24

rate results have been presented in Figs. 7 and 8 respectively along with experimental findings for comparison. It is observed that the simulated da/dN ~ ǻK points follow the experimental ones quite well. The number of cycles has been calculated from

22 20 18 5.50E+04

6.00E+04

6.50E+04

7.00E+04

No.of cycle(N)

7.50E+04

8.00E

Fig. 9. Comparison predicted (ANN) and experimentally obtained crack length with number of cycle (N) for load ratio 0.5 (7020 T7 alloy) 36 34

Predicted

Experimental

the simulated §¨ da ·¸ values by taking the first experimental ‘a’

© dN ¹

and ‘N’ values of 0.5 load ratio data set as the initial values and assuming an incremental crack length of 0.05mm in steps. The predicted a ~ N value of the ANN model has been compared with the experimental data in Figs. 9 and 10 respectively and a quantitative comparison of the prediction results have been presented in Table 3 for both the materials.

Crack length(a),mm

32 30

6. Conclusions 6. Conclusions

28 26 24 22 20 18 9.00E+04

9.50E+04

1.00E+05

1.05E+05

No.of cycle(N)

1.10E+05

Fig. 10. Comparison of predicted (ANN) and experimentally obtained crack length with number of cycle (N) for load ratio 0.5 (2024 T3 alloy)

5.2. Prediction model 5.2 Prediction by byANN ANN model Out of six experimental sets of load ratios (R = 0, 0.2, 0.4, 0.5, 0.6, 0.7. 0.8), the data set of load ratio 0.5 was left as validation set (VS). The adopted nine-layer perceptron (MLP) neural network model was applied to simulate the crack growth rate of the validation set for both the cases. The numbers of

Volume 1 • Issue 3 • 2009

In this work, fatigue crack propagation life of 7020 T7 and 2024 T3 aluminum alloys under the influence of load ratio was predicted by using artificial neural network (ANN). A data base consisting of six sets (R = 0, 0.2, 0.4, 0.6, 0.7. 0.8) of experimental data for each of the above alloys were used to train the ANN model. It was subsequently applied to predict the fatigue life for the unknown data set of R = 0.5. The model results were found to be in good agreement with the experimental findings. ANNs show great potential for predicting fatigue crack growth rate especially by interpolation within the tested range. However, its benefit is lost when the model is needed to extrapolate the available experimental data.

References References [1]

H. Al-Nashash, Y. Al-Assaf, B. Lvov, W. Mansoor, Laser speckle for materials classification utilizing wavelets and neural networks image processing techniques, Journal Materials Evaluation 59 (2001) 1072-1078.

137

[2]

P. Artymiak, L. Bukowski, J. Feliks, S. Narberhaus, H. Zenner, Determination of S-N curves with the application of artificial neural networks, Fatigue and Fracture of Engineering Materials and Structures 22 (1999) 723-728. [3] F. Aymerich, M. Serra, Prediction of fatigue strength of composite laminates by means of neural networks, Key Engineering Materials 144 (1998) 231-240. [4] W.F. Brown, J.E. Srawley, Plane strain crack toughness testing of high strength metallic materials, ASTM STP, American Society for Testing and Materials, Philadelphia, 1966, 1. [5] Y. Cheng, W.L. Huang, C.Y. Zhou, Artificial neural network technology for the data processing of on-line corrosion fatigue crack growth monitoring, International Journal of Pressure Vessels and Piping 76 (1999) 113-116. [6] S. Dinda, D. Kujawski, Correlation and prediction of fatigue crack growth for different R-ratios using Kmax and ǻK+ parameters, Engineering Fracture Mechanics 71 (2004) 1779-1790. [7] K. Donald, P.C. Paris, An evaluation of ǻKeff estimation procedures on 6060-T6 and 2024-T3 aluminum alloys, International Journal of Fatigue 21 (1999) 47-57. [8] W. Elber, The significance of fatigue crack closure. In: Damage tolerance in aircraft structures, ASTM STP 486, American Society for Testing and Materials, Philadelphia, 1971, 230-242. [9] M.E. Haque, K.V. Sudhakar, Prediction of corrosion-fatigue behavior of DP steel through artificial neural network, International Journal of Fatigue 23 (2001) 1-4. [10] S. Haykin, Neural Network, A Comprehensive Foundation, Prentice Hall, 1999. [11] R. Herzallah, Y. Al-Assaf, Control of non-linear and timevariant dynamic systems using neural networks, Proceedings of the 4th World Multiconference “Systemics, Cybernetics and Informatics”, Florida, 2000. [12] J.Y. Kang, J.H. Song, Neural network applications in determining the fatigue crack opening load, International Journal of Fatigue 20/1 (1998) 57-69.

138

[13] M. Klesnil, P. Lukas, Effect of stress cycle asymmetry on fatigue crack growth, Materials Science Engineering 9 (1972) 231-240. [14] D. Kujawski, A new (ǻK+Kmax) 0.5 driving force parameter for crack growth in aluminum alloys, International Journal of Fatigue 23 (2001) 733-740. [15] D. Kujawski, F. Ellyin, A fatigue crack growth model with load ratio effects, Engineering Fracture Mechanics 28 (1987) 367-378. [16] J.A. Lee, D.P. Almond, B. Harris, The use of neural networks for the prediction of fatigue lives of composite materials, Applied Science Manufacturing 30 (1999) 1159-1169. [17] C.S. Lee, W. Hwang, H.C. Park, K.S. Han, Failure of carbon/epoxy composite tubes under combined axial and torsional loading-1. Experimental results and prediction of biaxial strength by the use of neural networks, Composites Science and Technology 59 (1999) 1779-1788. [18] W. Mansoor, H. Al-Nashash, Y. Al-Assaf, Image classification using wavelets and neural networks, Proceedings of the 18th IASTED International Conference “Applied Informatics”, Austria, 2000. [19] R.M.V. Pidaparti, M.J. Palakal, Neural Network Approach to Fatigue-Crack-Growth Predictions under Aircraft Spectrum Loadings, Journal of Aircraft 32/4 (1995) 825-831. [20] T.T. Pleune, O.K. Chora, Using artificial neural networks to predict the fatigue life of carbon and low-alloy steels, Nuclear Engineering and Design 197 (2000) 1-12. [21] K Sadananda, A.K. Vasudevan, R.L. Holtz, E.U. Lee, Analysis of overload effects and related phenomenan, International Journal of Fatigue 21 (1999) 233-246. [22] V. Venkatesh, H.J. Rack, A neural network approach to elevated temperature creep-fatigue life prediction, International Journal of Fatigue 21 (1999) 225-234. [23] ASTM E647-00, Standard test method for measurement of fatigue crack growth rates, American Society for Testing & Materials, West Conshohocken.

READING DIRECT: www.archicmsse.org

Computational Materials Science and Surface Engineering

International Scientific Journal published quarterly by the Association of Computational Materials Science and Surface Engineering

2 0 0 9 • Vo l u m e 1 • Is s ue 3 • 133- 138

Application of artificial neural network for predicting fatigue crack propagation life of aluminum alloys J.R. Mohanty *, B.B. Verma, D.R.K. Parhi, P.K. Ray

Department of Metallurgical and Materials Engineering, National Institute of Technology, Rourkela 769008, India * Corresponding author: E-mail address: [email protected] Received in a revised form 08.05.2008

ABSTRACT

Purpose: In this work, fatigue crack propagation life of 7020 T7 and 2024 T3 aluminum alloys under the influence of load ratio was predicted by using artificial neural network (ANN). Design/methodology/approach: Numerous phenomenological models have been proposed for predicting fatigue life of the components under the influence of load ratio to take into account the mean load effect. Findings: In current research, an automatic prediction methodology has been adopted to estimate the constant amplitude loading fatigue life under the above condition by applying artificial neural network (ANN). Practical implications: ANNs show great potential for predicting fatigue crack growth rate especially by interpolation within the tested range. However, its benefit is lost when the model is needed to extrapolate the available experimental data. Originality/value: The predicted results are found to be in good agreement with the experimental findings when tested on two aluminum alloys 7020 T7 and 2024 T3 respectively. Keywords: Fatigue crack growth rate; Artificial Neural Network; Constant amplitude loading Reference to this paper should be given in the following way: J.R. Mohanty, B.B. Verma, D.R.K. Parhi, P.K. Ray, Application of artificial neural network for predicting fatigue crack propagation life of aluminum alloys, Archives of Computational Materials Science and Surface Engineering 1/3 (2009) 133-138.

ENGINEERING MATERIALS

1. Introduction 1. Introduction Most load bearing structural components generally contain defects / imperfections either as a result of manufacturing, fabrications or localized damage in service. Under different loading conditions, these defects coalesce and develop into large cracks, which propagate to critical size resulting catastrophic failure. The mere presence of a crack does not make a component or structure to be unreliable. Whatever may be the loading

condition, whether cyclic or sustained loading, it is necessary to know how long a crack would take to grow to a critical size at which the component or structure would become unsafe and fail. Therefore, the crack growth studies and life prediction procedure under fatigue loading is essential in order to extend the life of inservice sophisticated components so as to provide huge savings. It is known that load ratio (R) has a marked effect on fatigue crack growth rate. During last four decades, many prediction models have been proposed to incorporate the effect of R-ratio

© Copyright by International OCSCO World Press. All rights reserved. 2009

133

J.R. Mohanty, B.B. Verma, D.R.K. Parhi, P.K. Ray

including crack closure model [8], models based on residual compressive stress [13,15,] two-parameter driving force models [6,14] etc. However, automatic life prediction based on softcomputing methods such as artificial neural network (ANN), genetic algorithm (GA) etc is lacking. In the current investigation, an attempt has been made to predict fatigue life under the influence of R-ratio by using ANN. It is observed that the predicted results are in good agreement with the experimental findings.

K

f ( g ).

F Sa wB

(1)

where, f(g) = 1.12-0.231(a/w)+10.55(a/w)2-21.72(a/w)3+30.39(a/w)4 (2)

2. Experimental procedure 2. Experimental procedure This research was carried out on 7020 T7 and 2024 T3 aluminum alloys. A summary of chemical compositions and mechanical properties of both the alloys have been presented in Tables 1 and 2 respectively. The fatigue crack growth tests were performed using single edge notch tension (SENT) specimen with a thickness of 6.48 mm. The specimens were made in the LT plane, with the loading aligned in the longitudinal direction. Fig. 1 illustrates the major dimensions of the SENT samples used in the tests. A servo-hydraulic dynamic testing machine (Instron-8502) having a load capacity of 250 KN was used for the present investigation. Fatigue pre-cracking was introduced under mode I loading condition to an a/w ratio of 0.3 and were subjected to constant load amplitude test maintaining six load ratios (R) of 0, 0.2, 0.4, 0.6 and 0.8 respectively for both the materials. All fatigue tests were run at a frequency of 6 Hz with a sinusoidal wave form under ambient laboratory condition. Crack lengths were measured using a compliance method with a COD gauge and were also controlled using an optical method with a 20X magnification. The stress intensity factors at every instant ahead of the crack tip were calculated by using the following equations [4]:

Fig. 1. Geometry of the SENT specimen (dimensions in mm)

Table 1. Chemical Composition of 7020 T7 and 2024 T3 aluminum alloys Materials Al Cu Mg Mn 7020 T7 Main 0.05 1.2 0.43 constituent 2024 T3 90.7– 94.7 3.8 – 4.9 1.2–1.8 0.3 – 0.9

Table 2. Mechanical Properties of 7020 T7 and 2024 T3 aluminum alloys Young’s modulus Materials Tensile strength Yield strength (ıys) (E) (ıut) MPa MPa MPa

Fe 0.37

Si 0.22

Zn 4.6

Cr -

Others -

0.5

0.5

0.25

0.1

0.15

Poisson’s ratio (Ȟ)

Plane Strain Fracture toughness (KIC)

Elongation

MPa m 7020 T7

352.14

314.70

70,000

0.33

50.12

2024 T3

469.00

324.00

73,100

0.33

37.00

134

21.54 % in 40 mm 19 % in 12.7 mm

Archives of Computational Materials Science and Surface Engineering

Application of artificial neural network for predicting fatigue crack propagation life of aluminum alloys

3. Artificial neural 3. Artificial neuralnetwork networkapproach approach Artificial neural network (ANN) is a new class of computational intelligence system, useful to handle various complex problems with a capacity to learn by examples. It has proved to be a powerful and versatile soft-computing method which is quite efficient in modeling complex linear and non-linear relationships on the basis of experimental data in a number of engineering fields [1,3,11,16,18]. In recent years, ANN finds its application in the field of fatigue for various purposes [2,5,9,12,19,20,22]. It can be categories as feed forward or recurrent depending on the processing of data through the network. According to the learning rules, it can be further classified as supervised, unsupervised or reinforcement ANN. Among the various classifications, multi-layer perceptron (MLP) is the most popular ANN architecture as far as engineering application is concerned. MLPs are generally used with feed forward neural networks trained with error-back propagation algorithm (error minimization technique). Various non-linear activation functions such as sigmoidal, tanh or radial (Gaussian) are used to model the neuron activity.

4. esign ofofanan ANN model for crack 4. D Design ANN model for crack growth rate prediction growth rate prediction In the present investigation, a nine-layer perceptron ANN with back-propagation neural controller [10] has been developed. It has got one input layer, one output layer and seven hidden layers. The input layer has got three neurons, whereas one neuron has been associated with output layer. The neurons associated in the seven hidden layers are twelve, twenty four, hundred, thirty five and eight respectively. The neurons have been chosen empirically and taken in order so as to give the neural network a diamond shapes (Fig. 2).

The input parameters to the neural network controller are as follows: Stress intensity factor range = “sifr”; Maximum stress intensity factor = “msif”; Load ratio = “lr”. The output from the controller is: Crack growth rate = “cgr” The proposed ANN has been written in the C++ programming language and all the training tests have been performed on a personal computer. The activation function chosen in this work is the hyperbolic tangent function:

f ( x)

ex ex e x e x

(3)

During training, the network output șactual, may differ from the desired output șdesired as specified in the training pattern presented to the network. A measure of the performance of the network is the instantaneous sum-squared difference (error) between șdesired and șactual for the set of presented training patterns: 2 1 E rr ¦ T desired T actual 2 all training patterns

(4) where șactual represents crack growth rate (“cgr”) The two crack driving forces: stress intensity factor range (ǻK) and maximum stress intensity factor (Kmax) have been chosen as the two inputs as per ‘Unified Approach’ [6,7,14,21]. The third input is the load ratio (R) as the fatigue crack growth rate (da/dN) varies with the load ratio. The crack growth rate has been chosen as the output for the present ANN model. As far as normalization of input and output parameters are concerned, classical normalization, where the range is scaled between 0 and 1, may not be applicable in every ANN model. To make the input amenable for successful learning to minimize the overall sumsquared error, the two input parameters ǻK and Kmax have been normalized between 1 and 4, while the other one, load ratio (R) has been normalized between 1 and 3. Similarly the output § d a · ¨ ¸ © dN ¹

has been normalized between 0 and 3 for network training and testing. The inputs and outputs of the training sets (TS) have been constituted from 3× 65 experimental values of ǻK, Kmax and § da · data for each of the load ratios 0, 0.2, 0.4, 0.6, and 0.8 for ¨ ¸ © dN ¹ both the alloys.

5. Results 5. Results 5.1. Experimental 5.1 Experimentalresults results The experimental values of crack length versus number of cycles for various load ratios (R) have been illustrated in Figs. 3 and 4 respectively for both the materials. The crack growth rate,

§ da · has been calculated by incremental polynomial method as ¨ ¸ © dN ¹ Fig. 2. ANN architecture

Volume 1 • Issue 3 • 2009

per ASTM1. The results have been plotted against stress intensity factor (ǻK) in Figs. 5 and 6.

135

J.R. Mohanty, B.B. Verma, D.R.K. Parhi, P.K. Ray

36

R=0 R=0.2 R=0.4 R=0.5 R=0.6 R=0.8

34 32

28

0.95

1.05

1.15

1.25

1.35

1.45

1.55

-2.1

-2.6

log(da/dN)

Crack length(a),mm

30

0.85

26 24

-3.1

22

R=0

-3.6

R=0.2

20

R=0.4

18 16 3.00E+04 4.00E+04 5.00E+04 6.00E+04 7.00E+04 8.00E+04 9.00E+04 1.00E+05

-4.6

Fig. 3. Comparison of a ~ N curves for different load ratios (7020 T7 alloy) 36

30 28

Fig. 6. Comparison of da/dN ~ ǻK curves for different load ratios (2024-T3 alloy)

C rac k grow th rate(da/dN ).m m /c yc le

32

26 24 22 20 18 16 7.00E+04

log(del.K

2.00E-02

R=0 R=0.2 R=0.4 R=0.5 R=0.6 R=0.8

34

R=0.6 R=0.8

No. of cycle(N)

Crack length(a),mm

R=0.5

-4.1

9.00E+04

1.00E+05

1.10E+05

1.20E+05

Experimental

1.60E-02 1.40E-02 1.20E-02 1.00E-02 8.00E-03 6.00E-03 4.00E-03 2.00E-03 0.00E+00

8.00E+04

Predicted

1.80E-02

1.30E+05

10

15

No. of cycle(N)

Fig. 4. Comparison of a ~ N curves for different load ratios (2024 T3 alloy)

1.1

1.2

1.3

1.4

1.5

1.6

-1.7

log(da/dN)

-2.2

-2.7

-3.2

R=0

R=0.2

-3.7

R=0.4 R=0.5

-4.2

R=0.6 R=0.8

-4.7

log(del.K)

Fig. 5. Comparison of da/dN ~ ǻK curves for different load ratios (7020-T7 alloy)

136

Crack growth rate(da/dN),mm/cycle

1

25

30

35

Figure 7. Comparison of predicted (ANN) and experimental crack growth rate with stress intensity range (¨K) for load ratio 0.5 (7020 T7 alloy) 2.00E-02

0.9

20

Stress intensity factor range(del.K),Mpa.m^1/2

Predicted

1.80E-02

Experimental

1.60E-02 1.40E-02 1.20E-02 1.00E-02 8.00E-03 6.00E-03 4.00E-03 2.00E-03

0.00E+00

8.5

13.5

18.5

23.5

28.5

Stress intensity factor range(del.K),Mpa.m^1/2

33.5

Fig. 8.Comparison of predicted (ANN) and experimental crack growth rate with stress intensity range (¨K) for load ratio 0.5 (2024 T3 alloy)

Archives of Computational Materials Science and Surface Engineering

Application of artificial neural network for predicting fatigue crack propagation life of aluminum alloys

Table 3. Load scenarios and model results of the tested specimens Test specimen Fmax Fmin R ai (KN) (KN) (mm)

af (mm)

N Af

N Ef

% error in

% error in

Kcycle

Kcycle

N Af

N Ef

7020 T7

7.944

3.972

0.5

18.3

35.1

75.344

78.265

-4.365

-0.658

2024 T3

7.204

3.602

0.5

18.3

35.4

110.920

112.879

-2.099

-0.370

34

hidden neurons, minimum error and number of iterations were chosen empirically as 7, 1 u 10 6 and 4, 48, 000. The input parameters, stress intensity factor range (ǻK), maximum stress intensity factor (Kmax) and load ratio have been fed to the trained ANN model in order to predict the corresponding crack growth

Predicted

Experimental

Crack length(a),mm

32 30 28

rate §¨ da ·¸ for the validation set. The predicted crack growth

26

© dN ¹

24

rate results have been presented in Figs. 7 and 8 respectively along with experimental findings for comparison. It is observed that the simulated da/dN ~ ǻK points follow the experimental ones quite well. The number of cycles has been calculated from

22 20 18 5.50E+04

6.00E+04

6.50E+04

7.00E+04

No.of cycle(N)

7.50E+04

8.00E

Fig. 9. Comparison predicted (ANN) and experimentally obtained crack length with number of cycle (N) for load ratio 0.5 (7020 T7 alloy) 36 34

Predicted

Experimental

the simulated §¨ da ·¸ values by taking the first experimental ‘a’

© dN ¹

and ‘N’ values of 0.5 load ratio data set as the initial values and assuming an incremental crack length of 0.05mm in steps. The predicted a ~ N value of the ANN model has been compared with the experimental data in Figs. 9 and 10 respectively and a quantitative comparison of the prediction results have been presented in Table 3 for both the materials.

Crack length(a),mm

32 30

6. Conclusions 6. Conclusions

28 26 24 22 20 18 9.00E+04

9.50E+04

1.00E+05

1.05E+05

No.of cycle(N)

1.10E+05

Fig. 10. Comparison of predicted (ANN) and experimentally obtained crack length with number of cycle (N) for load ratio 0.5 (2024 T3 alloy)

5.2. Prediction model 5.2 Prediction by byANN ANN model Out of six experimental sets of load ratios (R = 0, 0.2, 0.4, 0.5, 0.6, 0.7. 0.8), the data set of load ratio 0.5 was left as validation set (VS). The adopted nine-layer perceptron (MLP) neural network model was applied to simulate the crack growth rate of the validation set for both the cases. The numbers of

Volume 1 • Issue 3 • 2009

In this work, fatigue crack propagation life of 7020 T7 and 2024 T3 aluminum alloys under the influence of load ratio was predicted by using artificial neural network (ANN). A data base consisting of six sets (R = 0, 0.2, 0.4, 0.6, 0.7. 0.8) of experimental data for each of the above alloys were used to train the ANN model. It was subsequently applied to predict the fatigue life for the unknown data set of R = 0.5. The model results were found to be in good agreement with the experimental findings. ANNs show great potential for predicting fatigue crack growth rate especially by interpolation within the tested range. However, its benefit is lost when the model is needed to extrapolate the available experimental data.

References References [1]

H. Al-Nashash, Y. Al-Assaf, B. Lvov, W. Mansoor, Laser speckle for materials classification utilizing wavelets and neural networks image processing techniques, Journal Materials Evaluation 59 (2001) 1072-1078.

137

[2]

P. Artymiak, L. Bukowski, J. Feliks, S. Narberhaus, H. Zenner, Determination of S-N curves with the application of artificial neural networks, Fatigue and Fracture of Engineering Materials and Structures 22 (1999) 723-728. [3] F. Aymerich, M. Serra, Prediction of fatigue strength of composite laminates by means of neural networks, Key Engineering Materials 144 (1998) 231-240. [4] W.F. Brown, J.E. Srawley, Plane strain crack toughness testing of high strength metallic materials, ASTM STP, American Society for Testing and Materials, Philadelphia, 1966, 1. [5] Y. Cheng, W.L. Huang, C.Y. Zhou, Artificial neural network technology for the data processing of on-line corrosion fatigue crack growth monitoring, International Journal of Pressure Vessels and Piping 76 (1999) 113-116. [6] S. Dinda, D. Kujawski, Correlation and prediction of fatigue crack growth for different R-ratios using Kmax and ǻK+ parameters, Engineering Fracture Mechanics 71 (2004) 1779-1790. [7] K. Donald, P.C. Paris, An evaluation of ǻKeff estimation procedures on 6060-T6 and 2024-T3 aluminum alloys, International Journal of Fatigue 21 (1999) 47-57. [8] W. Elber, The significance of fatigue crack closure. In: Damage tolerance in aircraft structures, ASTM STP 486, American Society for Testing and Materials, Philadelphia, 1971, 230-242. [9] M.E. Haque, K.V. Sudhakar, Prediction of corrosion-fatigue behavior of DP steel through artificial neural network, International Journal of Fatigue 23 (2001) 1-4. [10] S. Haykin, Neural Network, A Comprehensive Foundation, Prentice Hall, 1999. [11] R. Herzallah, Y. Al-Assaf, Control of non-linear and timevariant dynamic systems using neural networks, Proceedings of the 4th World Multiconference “Systemics, Cybernetics and Informatics”, Florida, 2000. [12] J.Y. Kang, J.H. Song, Neural network applications in determining the fatigue crack opening load, International Journal of Fatigue 20/1 (1998) 57-69.

138

[13] M. Klesnil, P. Lukas, Effect of stress cycle asymmetry on fatigue crack growth, Materials Science Engineering 9 (1972) 231-240. [14] D. Kujawski, A new (ǻK+Kmax) 0.5 driving force parameter for crack growth in aluminum alloys, International Journal of Fatigue 23 (2001) 733-740. [15] D. Kujawski, F. Ellyin, A fatigue crack growth model with load ratio effects, Engineering Fracture Mechanics 28 (1987) 367-378. [16] J.A. Lee, D.P. Almond, B. Harris, The use of neural networks for the prediction of fatigue lives of composite materials, Applied Science Manufacturing 30 (1999) 1159-1169. [17] C.S. Lee, W. Hwang, H.C. Park, K.S. Han, Failure of carbon/epoxy composite tubes under combined axial and torsional loading-1. Experimental results and prediction of biaxial strength by the use of neural networks, Composites Science and Technology 59 (1999) 1779-1788. [18] W. Mansoor, H. Al-Nashash, Y. Al-Assaf, Image classification using wavelets and neural networks, Proceedings of the 18th IASTED International Conference “Applied Informatics”, Austria, 2000. [19] R.M.V. Pidaparti, M.J. Palakal, Neural Network Approach to Fatigue-Crack-Growth Predictions under Aircraft Spectrum Loadings, Journal of Aircraft 32/4 (1995) 825-831. [20] T.T. Pleune, O.K. Chora, Using artificial neural networks to predict the fatigue life of carbon and low-alloy steels, Nuclear Engineering and Design 197 (2000) 1-12. [21] K Sadananda, A.K. Vasudevan, R.L. Holtz, E.U. Lee, Analysis of overload effects and related phenomenan, International Journal of Fatigue 21 (1999) 233-246. [22] V. Venkatesh, H.J. Rack, A neural network approach to elevated temperature creep-fatigue life prediction, International Journal of Fatigue 21 (1999) 225-234. [23] ASTM E647-00, Standard test method for measurement of fatigue crack growth rates, American Society for Testing & Materials, West Conshohocken.

READING DIRECT: www.archicmsse.org